Upload
others
View
4
Download
0
Embed Size (px)
BUCKLING ANALYSIS OF SWCNT
REINFORCED COMPOSITE PLATE
A Report Submitted
In Partial Fulfilment of the Requirements for the degree of
Bachelor of Technology in Mechanical Engineering
Sourava Jyoti Nayak
ROLL NO: 110ME0316
(Department Of Mechanical Engineering)
Under the Supervision of
Prof. Subrata Kumar Panda
Department Of Mechanical Engineering
National Institute Of Technology Rourkela
Rourkela-769008
brought to you by COREView metadata, citation and similar papers at core.ac.uk
provided by ethesis@nitr
BUCKLING ANALYSIS OF SWCNT
REINFORCED COMPOSITE PLATE
A Report Submitted
In Partial Fulfilment of the Requirements for the degree of
Bachelor of Technology in Mechanical Engineering
Sourava Jyoti Nayak
ROLL NO: 110ME0316
(Department Of Mechanical Engineering)
Under the Supervision of
Prof. Subrata Kumar Panda
Department Of Mechanical Engineering
National Institute Of Technology Rourkela
Rourkela-769008
NATIONAL INSTITUTE OF TECHNOLOGY ROURKELA – 769008, ODISHA
INDIA
CERTIFICATE
This is to certify that the thesis entitled, “BUCKLING ANALYSIS OF SWCNTREINFORCED
COMPOSITE PLATES” submitted by Mr Sourava Jyoti Nayak in partial fulfilment of the
requirement for the award of Bachelor of Technology Degree in Mechanical Engineering with
specialization in Mechanical Engineering at the National Institute of Technology, Rourkela
(Deemed University) is an authentic work carried out by him under my supervision and guidance.
To the best of my knowledge, the matter embodied in the thesis has not been submitted to
any other University/ Institute for the award of any degree or diploma.
Dr. S.K. Panda
Department Of Mechanical Engineering
NIT Rourkela
Acknowledgment
I would like to express my gratitude to my esteemed guide, Dr. Subrata Kumar Panda Assistant
Professor (Department of Mechanical Engineering, NIT Rourkela) for his encouragement,
advice, mentoring and research support throughout my project work . His technical and editorial
advice was essential for the completion of this dissertation. He has been a great inspiration for me
and has helped me in every possible manner throughout this project.
I would also like to thank Mr. Vishesh Ranjan Kar and Mr. Vijay Kumar Singh, Ph.D. scholars
of Department of Mechanical Engineering, NIT Rourkela for guiding me throughout the
analysis part of this project by virtue of their vast experience to work with ANSYS software.
I also thank all my friends, who have directly or indirectly helped me in my project work and in
the completion of this report.
Sourava Jyoti Nayak (110me0316)
Department of Mechanical Engineering
NIT Rourkela
Abstract
This work presents the buckling analysis of functionally graded single walled carbon nanotubes
reinforced composite plates under in-plane mechanical loads. The effective material properties of
uniformly distributed carbon nanotubes are obtained using Mori–Tanaka approach and extended
rule of mixtures. The buckling load has been obtained numerically with the help of commercial
finite element package ANSYS using ANSYS parametric design language code. The convergence
behaviour of the developed model has been checked and validated by comparing the responses
with those available literature. Effect of different geometrical parameters such as aspect ratio and
side to thickness ratio have been studies and discussed in details.
Key words: SWCNT, FEM, ANSYS, Laminated composite, Bucklin
CONTENTS
Chapter 1…………………………………………………………………01-04
Introduction and literature review
Chapter 2…………………………………………………………………05-12
Theoretical formulation and modelling
Chapter 3…………………………………………………………………13-18
Experimental study
Chapter 4…………………………………………………………………19-22
Results and discussions
Chapter 5…………………………………………………………………23-24
Conclusion
Chapter 6……………………………………………………………..…..25-27
References
List of figures:
Serial No Figure Page
1 Geometrical representation of SHELL 281 4
2 FGCNT plate model with uniformly distributed CNT [9] 9
3 FGCNT plate model 10
4 Convergence behaviour of nondimensional buckling load
parameter
11
5 Effect of thickness ratio on buckling load parameter 12
6 Effect of aspect ratio on buckling load parameter
12
7(a) - 7(d) Buckling Modes 12
List of Tables:
Serial No Table Page
1 Comparison of critical buckling load 11
1
Introduction and literature review
Carbon nanotubes (CNTs) are carbon allotropes whose structure resembles that of a cylinder. The
length to diameter ratio of CNT’s can be in excess of thousands. It is well known from various
experiments conducted by the researcher and claimed that the aspect ratio (l/d) exceed 1.32×108 to
1. These carbon atoms which are cylindrical in shape have very unusual properties which find
application in electronics, optics, nanotechnology and other areas of science and engineering.
These tubes possess extremely high thermal conductivity and electrical and mechanical properties
and find application in material science and engineering. Nanotubes are used in tiny quantities and
in microscopic proportions for common items like golf balls and in military application like gun
barrels.
The basic structure of a nanotube resembles that of a fullerene, it is like long hollow walls which
are formed by layers of carbon one atom thick which is called graphene. These tubes vary in
properties depending upon the angle of rolling and the rolling radius. The angle of rolling assumes
prime importance in determining the properties of the CNT and is called as chiral angle. Nanotubes
are mainly classified as single walled and multi walled nanotubes (SWCNT/MWCNT). All
nanotube molecules are held together by covalent forces which are also known as Vander Walls
forces. Quantum chemistry and orbital hybridization can be used to describe the chemical structure
of CNT’s and it is composed of completely sp2 bonds, like graphite.
There are numerous applications of CNT’s which vary from use in miniscule applications
involving nanotechnology to providing strength to gigantic structures. Breakthroughs carried out
by Ray H. Baughman at the Nano Tech Institute has proposed that MWCNT and SWCNT can
yield substances with great toughness which has been previously unheard of. Many researchers
have carried out experiments to reinforce composites of CNT’s. Generally mechanical, thermal
and electrical properties of composite structures greatly depend on the added reinforcement, and
the elasticity and tension strength of CNTs may give strong and stiff composite structures, such as
shells, beams and plates.
Buckling of structural parts and equipment is a common failure mode. Buckling is a geometrical
instability, which leads to a catastrophic failures. Buckling is characterized by a sudden failure of
2
a structural member subjected to high compressive stress, where the actual compressive stress at
the point of failure is less than the ultimate compressive stresses that the material is capable of
withstanding. Numerous studies have been conducted to study and describe the buckling behaviour
of composites.
Many studies have been reported in literature to predict the buckling strength of functionally
graded carbon nanotube (FGCNT) under mechanical loading.
Most examinations of carbon nanotubes-fortified composites (CNTRC) have concentrated on
material properties and specialists have uncovered that mechanical, electrical and warm properties
of polymer composites could be respectably enhanced by including little measures of Cnts.
Odegard et al. [1] displayed a constitutive displaying of nanotubes-fortified polymer composites
with nanotubes/ polymer interface displayed as a powerful continuum fiber by utilizing a
proportional-continuum model. Gary et al. [2] acquired the powerful flexible properties of
CNTRCs through an assortment of micromechanics systems with the powerful properties of CNTs
ascertained using a composite barrels micromechanics method as a first venture in a two-stage
process. Fidelus et al. [3] analyzed the thermo-mechanical properties of epoxy-based
nanocomposites focused around low weight parts of arbitrarily arranged single- and multi-walled
carbon nanotubes. Han and Elliot [4] displayed established sub-atomic motion (MD) enactments’
of model polymer/CNT composites developed by implanting a solitary divider (10, 10) CNT into
two separate indistinct polymer networks. By utilizing MD technique, the stress–strain conduct of
carbon nanotube-fortified Epon862 composites was additionally considered by Zhu et al
[5].Despite the fact that these studies are truly helpful, a definitive reason for improvement of this
propelled material is to investigate potential provisions of CNTs in genuine structures, for
example, CNT-fortified pillars, plates or shells. Wuite and Adali [6] examined diversion and stress
practices of nanocomposite fortified shafts utilizing a multiscale investigation. Their effects
indicated that fortification by including a little extent of nanotube prompts noteworthy change in
shaft solidness. Vodenitcharova and Zhang [7] displayed investigates of immaculate bowing and
twisting-prompted neighbourhood clasping of a nanocomposite shaft focused around a continuum
mechanical model and found that solitary-walled carbon nanotube (SWCNT) clasps at littler
curving edges and more excellent straightening degrees in thicker framework layers. Formica et
al. [8] explored vibration practices of CNTRC plates by utilizing an identical continuum model
focused around the Eshelby–Mori–Tanaka approach.
3
Based on the above review, it is clear that the buckling behaviour of FGCNT composite have been
reported in open literature but the number is very few. Hence, here we aim to analyse the
mechanical behaviour of FGCNT composite plates under mechanical loading. As a first step,
FGCNT model has been developed in ANSYS using ANSYS parametric design language code
(APDL). The effective material properties of the FGCNT has been obtained using Mori-Tanaka
extended rule of mixture. The model has been discretised using the SHELL281 element from
ANSYS library. The convergence behaviour of the developed model has been checked and
compared with those available literature. Some new results are also computed based on the
different (thickness ratio and aspect ratio) parameters.
4
Mathematical Formulation
For the modelling purpose, a SHELL 281 element as shown in Fig. 1 is selected from the ANSYS
13.0 element library. This is an element having eight nodes and contains six degrees of freedom(
three of the six degrees belongs to translations along x , y and z axes and the remaining three
degrees belongs to rotations along x,y and z axes) per node. It works on shear deformation theory
of the first order and is most appropriate for linear, large rotation, and/or large strain nonlinear
applications. The formulation of is based on logarithmic strain and true stress measures.
Fig. 1 Geometrical representation of SHELL281 [10]
x0 = Element x-axis if element orientation is not provided.
x1 = Element x-axis if element orientation is provided.
It is well known that the mathematical model have been used the FSDT to model in ANSYS and
the displacement field is conceded as [10]:
u(x, y, z) = u0(x,y)+ zθx(x,y)
v(x, y, z) = v0(x,y) + zθy(x,y) ……………………………………….(1)
w(x, y, z) =w0(x,y) +zθz(x,y)
The displacements u,v and w can be represented in terms of shape functions (Ni) as [10]:
5
δ= 1
j
i ii
N …………………………………………………..(2)
where δi = [u0i v0i w0i θxiθyiθzi]T
The shape functions for the 8 noded (j=8) shell element (SHELL 281) are given by [10] :
N1= 1/4×(1 – ζ) (1 – η) ( – ζ – η – 1) ; N2= 1/4×(1 + ζ) (1 – η) (ζ – η – 1)
N3= 1/4×(1 + ζ) (1 + η) (ζ + η – 1) ; N4= 1/4×(1 – ζ) (1 + η) ( – ζ + η – 1) ……..(3)
N5= 1/2×(1 – ζ 2) (1 – η) ; N6= 1/2×(1 + ζ) (1 – η2)
N7= 1/2×(1 – ζ 2) (1 + η) ; N8= 1/2×(1 – ζ) (1 – η2)
Strains can be got by derivation of displacements which can be shown as:
, , , , , , , , ,x y z y x z y x zu v w u v v w w u
where {ε}={ εx , εy , εz , γxy , γyz , γzx }T is the strain matrix containing normal and shear strain
components of the mid-plane in in-plane and out of plane direction.
The strain components are now rearranged in the following steps.
The in-plane strain vector is given by [10]:
0
0
0
x x x
y y y
xy xy xy
z
…………………………………………………(4)
The transverse strain vector is given by [10] :
0
0
0
zz z
yz yz yz
xz xz xz
z
…………………………………………………(5)
The deformation components are explained as [10] :
6
0
00
00 0
;
x
xo z
y
y yz
xy xzyx
u
xx
v
y y
u v
y x y x
…………………………………………(6)
00
00
0
;
zzo z
zyz y yz
xz xzz
x
w
y y
w
xx
…………………………………………(7)
The strain vector are represented in terms of nodal displacement vector
{ε}= [B] {δ}…………………………………………(8)
[B] is the strain displacement matrix having shape functions and their derivatives and { } is the
nodal displacement vector.
For a laminate, the stress-strain relationship with respect to its reference plane can be expressed
as:
{ } = [D]{ε} …………………………………………(9)
where, { } and {ε} is the stress and strain vector respectively and [D] is the rigidity matrix
containing the effective material properties of the orthotropic matrix of the composite plate.
The element stiffness matrix [K] may be easily obtained by virtual work method which can be
expressed as [10] :
[K] =
1 1
1 1
[B]T [D] [B]|J|dζdη…………………………………………(10)
where, |J| : Determinant of the Jacobian matrix, [N]: Shape function matrix and [m] : the
inertia matrix.
7
The integration has been done using the Gaussian quadrature method.
The nodal displacements can be written in the form of their shape functions and corresponding
nodal values as follows [10]:
8 8 8 8 8 80 0 0 0 0 0 0 0 0
1 1 1 1 1 1
, , , , ,i i i i i i x i xi y i yi z i zi
i i i i i i
u N u v N v w N w N N N
The above expression can be reshown in ith nodal displacement as follows :
* 0 0 0 0 0 0
i i i i xi yi wiu v w …………………………………………(11)
*
i i iN …………………………………………(12)
where
0 0 0 0 0
0 0 0 0 0
0 0 0 0 0
0 0 0 0 0
0 0 0 0 0
0 0 0 0 0
i
i
i
i
i
i
i
N
N
NN
N
N
N
…………………………………………(13)
Substituting the value of nodal displacement in strain, strain energy we will get
i i iB
1
[ ] [ ][ ]2
T T
i i i i miU B D B dA F …………………………………………(14)
where [ ]iB : strain displacement relation matrix,
m
F : mechanical force, respectively.
8
The final form of the equation can be obtained by minimizing the total potential energy (TPE) as
follows:
0
Where, is the total potential energy.
[ ]{ } { }mK F
where, [M] and [K] are the global mass and stiffness matrix.
The buckling equation can be obtained for the laminated shell/plate and conceded as [10] :
[ ]{ } { }mK F …………………………………………(15)
In this study eigenvalue type of buckling has studied and the eigenvalue equation will be obtained
by dropping the force vectors and considering their effects in geometry the new form of the Eq.
(21) will be expressed as [10] :
[ ] 0cr GK K …………………………………………(16)
where [KG] =the geometric stiffness matrix
cr = critical mechanical load at which the structure buckles.
Carbon nanotube reinforced composite plates
An ANSYS model of UD -CNTRC plate has been developed by defining the length a, width b,
and thickness h. The compelling material properties of the two-stage nano composites, mixture of
CNTs and an orthotropic polymer as per the Mori–Tanaka rule of mixture
(1a)
(1b)
(1c)
where, 11
CNTE , 22
CNTE and 12
CNTG indicate the young’s modulus and shear modulus of SWCNTS
, respecting and mE and mG represent the properties of the orthotropic matrix. Similarly, V*
CNT is
the volume part of the carbon nanotube and VCNT is the volume portion of the matrix.
11 11
2
22 22 12
3
12 12
CNT m
CNT m
CNT m m
CNT CNT m
CNT m
CNT m
E V E V E
V V V
E E E E
V V
G G G
9
CNTV=
V CNT
(UD CNTRC) 2(a)
where,( / ) ( / )
CNTCNT CNT m CNT m
CNT CNT
WV
W W
2(b)
where, CNTW =weight fraction of the CNT in the composite plate
CNT = Densities of the carbon nanotubes
m = Densities of the matrix.
12 12V ..........................................................................3( )CNT m
CNT mV a
................................................................................3( )CNT m
CNT mV V b
11 11
CNT m
CNT mV V …………………………………………………...3(c)
11 22 12 22 m 12 11(1 ) (1 )VCNT CNT m m
CNTV …………………..3(d)
where,12
CNT and m are Poisson’s ratio of CNT and matrix and11
CNT ,22
CNT , m are the thermal
expansion coefficients in 1 and 2-directions of the CNT and matrix, respectively. The 12 remains
invariable along the transverse direction of the CNTRC plate. The details of UD FGCNT is
presented in Fig. 2
Fig.2. FGCNT plate model with uniformly distributed CNT [9]
10
Results and Discussion
In this section, the FGCNT model of uniformly distributed (UD) composite plate have been
developed using APDL code in ANSYS. As discussed a plate having dimensions a = b = 20 mm
and h = 2 mm and the effective modulus of elasticity of matrix (Em) = 2.1109 N/mm2 have been
developed and presented in Fig. 3.
Fig. 3. FGCNT plate model
The following simply supported boundary conditions are used for the analysis [9]:
0 0 0yv w at x = 0 and x = a
0 0 0xu w at y = 0 and y = b
Convergence and Comparison Study
In order to check the convergence behaviour of the present model, the present model has been
developed in ANSYS and presented in Fig.4. It is clearly observed that the present results are
converging well with mesh refinement. In continuation to that, the nondimensional critical
buckling load parameters are computed using the present APDL code and the comparison study
has been presented in Table 1. The material and geometrical parameters are same as the reference.
The ANSYS model is showing very good agreement with that of the reference.
11
10X10 12X12 14X14 16X16 18X18 20X20 22X22 24X24
0.0
0.5
1.0
1.5
2.0
2.5
3.0
3.5
4.0
Cri
tica
l bu
cklin
g lo
ad
pa
ram
ete
r
Mesh size
a/h=100
Fig.4 Convergence behaviour of nondimensional buckling load parameter
Table 1. Comparison of critical buckling load.
Mode No. Present crN Reference [9] Percentage of difference
1 27.44 28.4768 3.78
2 27.46 28.8410 5.03
3 27.64 29.5768 7.01
4 28.94 30.1219 4.08
Numerical Illustration
Some new results are computed for FGCNT composite plate for thickness ratio and aspect ratio
and presented in Fig. 5 and 6, respectively. It is observed that the buckling load parameters
increases as the thickness ratio increases and the decreases with aspect ratio. In addition to that
four different buckling mode shapes are presented in Fig. 7 (a), (b), (c) and (d), respectively.
12
0 20 40 60 80 100
0.3
0.4
0.5
0.6
0.7
0.8
0.9 Buckling LoadC
ritica
l b
ucklin
g lo
ad
pa
ram
ete
r
Thickness ratio
0.8 1.0 1.2 1.4 1.6 1.8 2.0 2.2 2.4 2.6
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
Buckling Load
Cri
tica
l b
ucklin
g lo
ad
pa
ram
ete
r
Aspect ratio
Fig. 5. Effect of thickness ratio on buckling
load parameter
Fig. 6. Effect of aspect ratio on buckling load
parameter
Fig. 7 (a). 1st Mode Fig. 7(b). 2nd Mode
Fig. 7(c). 1st Mode Fig. 7(d). 1st Mode
13
Conclusions:
In this study, the nondimensional buckling load parameter have been obtained numerically. The
model has been developed in ANSYS using APDL code. The convergence and comparison
behaviour of the developed model has been checked. Some new results are computed for thickness
ratio and aspect ratio. The results are following the expected line.
14
References
1] Odegard GM, Gates TS, Wise KE, Park C, Siochi EJ. Constitutive modeling of nanotube–
reinforced polymer composites. Compos Sci Technol 2003;63:1671–87.
[2] Seidel GD, Lagoudas DC. Micromechanical analysis of the effective elastic properties of
carbon nanotube reinforced composites. Mech Mater 2006;38:884–907.
[3] Fidelus JD, Wiesel E, Gojny FH, Schulte K, Wagner HD. Thermo-mechanical properties of
randomly oriented carbon/epoxy nanocomposites. Composites:Part A 2005;36:1555–61.
[4] Han Y, Elliott J. Molecular dynamics simulations of the elastic properties of polymer/carbon
nanotube composites. Comput Mater Sci 2007;39:315–23.
[5] Zhu R, Pan E, Roy AK. Molecular dynamics study of the stress–strain behaviour of carbon-
nanotube reinforced Epon 862 composites. Mater Sci Eng, A 2007;447:51–7.
[6] Wuite J, Adali S. Deflection and stress behaviour of nanocomposite reinforced beams using a
multiscale analysis. Compos Struct 2005;71:388–96.
[7] Vodenitcharova T, Zhang LC. Bending and local buckling of a nanocomposite beam reinforced
by a single-walled carbon nanotube. Int J Solids Struct 2006;43:3006–24.
[8] Formica G, Lacarbonara W, Alessi R. Vibrations of carbon nanotube-reinforced composites. J
Sound Vib 2010;329:1875–89.
[9] Z.X. Lei, K.M. Liew, J.L. Yu, Buckling analysis of functionally graded carbon nanotube-
reinforced composite plates using the element-free kp-Ritz method.
[10] Santanu Kumar Sahu, Static and Buckling analysis of Laminated Sandwich Plates with
Orthotropic Core using FEM, Department of Mechanical Engg., NIT Rourkela,Odisha,India.